Laksono, David Wahyu (2009) PENGARUH PENGGANTIAN SEBAGIAN AGREGAT PASIR DENGAN AGREGAT DARI LIMBAH PLASTIK DALAM PEMBUATAN BATAKO TERHADAP KARAKTERISTIK DAN KUAT TEKAN BATAKO DENGAN METODE PRESSING. (study penelitian). Other thesis, University of Muhammadiyah Malang.
Download (54kB) | Preview
Addition of aggregate of plastic waste in composition of batako represent step exploiting of plastic waste become goods which good for that is additional materials at batako. This research is meant to know the nature of characteristic of batako cover absorpsion, specific gravity, strength and porosity depress with addition of plastic aggregate at planned composition variation of. obtained benefit of this research is can know by influence of addition of plastic aggregate in making of batako, can develop science in making of batako. Batako of the size 30 cm × 10 cm × 13 cm made [by] counted 60 with aggregate variation [of] of plastic waste equal to 0%, 10%, 20%, 30%, and 40% each made 3 test object. Test object given for the treatment of cement mixture variable or : sand : water ( 1:2:0,6, 1:3:0,6, 1:4:0,6, 1:5:0,6). Method making of batako that is by and pressing of pressing used equal to 20 Mpa. From result of this research is got by various classification storey; level Quality of, quality 1 there are [at] type batako of I(1:2:0,6) with plastic aggregate mixture 0% until 30%, type batako of II(1:3:0,6) with plastic aggregate mixture 0% and 10%, type batako of III(1:4:0,6) with plastic aggregate mixture 0% and 10%, type batako of IV(1:5:0,6) with plastic aggregate mixture 0%. quality 2 there are [at] type batako of I(1:2:0,6) with plastic aggregate mixture 40%, type batako of II(1:3:0,6) with plastic aggregate mixture 20%, type batako of III(1:4:0,6) with plastic aggregate mixture 20%, type batako of IV(1:5:0,6) with plastic aggregate mixture 10% and 20%. quality 3 there are at type batako of II(1:3:0,6) with plastic aggregate mixture 30% and 40%, type batako of III(1:4:0,6) with plastic aggregate mixture 30% and 40%, type batako of IV(1:5:0,6) with plastic aggregate mixture 30% and 40%. So that batako earn dipakia and peaceful for construction material. With plastic aggregate mengunakan of makn strong depress which is got progressively lower because plastic aggregate don't have energy fasten, absorpsion of batako excelsior because weakening of tying between aggregate form bubble and pore many so that absorbtion of ever greater batako, porosity of batako ever greater because tying between weak aggregate so that cavity terdapan so that batako progressively porous. and specific gravity batako become to lower because influence specific gravity light plastic aggregate so that influence to specific gravity batako.
|Item Type:||Thesis (Other)|
|Subjects:||T Technology > TA Engineering (General). Civil engineering (General)|
|Divisions:||Faculty of Engineering > Department of Civil Engineering|
|Depositing User:||Anggit Aldila|
|Date Deposited:||15 Jun 2012 07:12|
|Last Modified:||15 Jun 2012 07:12|
Actions (login required)